Microstructural Evolution in the 2219 Aluminum Alloy ... /67531/metadc... The microstructural...
Embed Size (px)
Transcript of Microstructural Evolution in the 2219 Aluminum Alloy ... /67531/metadc... The microstructural...
R.O. Kaibyshev, I.M. Safarov, D.R. Lesuer
March 29, 2000
Microstructural Evolution in the 2219 Aluminum Alloy During Severe Plastic Deformation
U.S. Department of Energy
Lawrence Livermore National Laboratory
DISCLAIMER This document was prepared as an account of work sponsored by an agency of the United States Government. Neither the United States Government nor the University of California nor any of their employees, makes any warranty, express or implied, or assumes any legal liability or responsibility for the accuracy, completeness, or usefulness of any information, apparatus, product, or process disclosed, or represents that its use would not infringe privately owned rights. Reference herein to any specific commercial product, process, or service by trade name, trademark, manufacturer, or otherwise, does not necessarily constitute or imply its endorsement, recommendation, or favoring by the United States Government or the University of California. The views and opinions of authors expressed herein do not necessarily state or reflect those of the United States Government or the University of California, and shall not be used for advertising or product endorsement purposes. Work performed under the auspices of the U. S. Department of Energy by the University of California Lawrence Livermore National Laboratory under Contract W-7405-Eng-48.
This report has been reproduced directly from the best available copy.
Available to DOE and DOE contractors from the
Office of Scientific and Technical Information P.O. Box 62, Oak Ridge, TN 37831
Prices available from (423) 576-8401 http://apollo.osti.gov/bridge/
Available to the public from the
National Technical Information Service U.S. Department of Commerce
5285 Port Royal Rd., Springfield, VA 22161 http://www.ntis.gov/
Lawrence Livermore National Laboratory
Technical Information Department’s Digital Library http://www.llnl.gov/tid/Library.html
MICROSTRUCTURAL EVOLUTION IN THE 2219 ALUMINUM ALLOY DURING SEVERE PLASTIC DEFORMATION
R.O. Kaibyshev1, I.M.Safarov1, D.R.Lesuer2
1Institute for Metals Superplasticity Problems, Khalturina 39, Ufa 450001, Russia 2 Lawrence Livermore National Laboratory, L-342 P.O. Box 808, Livermore, CA 94551, USA
Keywords: microstructural evolution, severe plastic deformation, cell structure, dislocation rich bands, nanocrystalline structure.
Numerous investigations have demonstrated that intense plastic deformation is an attractive procedure for producing an ultrafine grain size in metallic materials. Torsional deformation under high pressure  and equal-channel angular extrusion  are two techniques that can produce microstructures with grain sizes in the submicrometer and nanometer range. Materials with these microstructures have many attractive properties. The microstructures formed by these two processing techniques are essentially the same and thus the processes occurring during deformation should be the same.
Most previous studies have examined the final microstructures produced as a result of severe plastic deformation and the resulting properties. Only a limited number of studies have examined the evolution of microstructure [3-6]. As a result, some important aspects of ultra-fine grain formation during severe plastic deformation remain unknown. There is also limited data on the influence of the initial state of the material on the microstructural evolution and mechanisms of ultra- fine grain formation. This limited knowledge base makes optimization of processing routes difficult and retards commercial application of these techniques.
The objective of the present work is to examine the microstructure evolution during severe plastic deformation of a 2219 aluminum alloy. Specific attention is given to the mechanism of ultrafine grain formation as a result of severe plastic deformation.
Materials and Experimental Technique
The 2219 aluminum alloy with the chemical composition Al-6.4%Cu-0.3%Mn-0.18%Cr-0.19%Zr- 0.06%Fe was cast at the Kaiser Aluminum - Center for Technology by direct chill casting. The alloy was then homogenized at 5300C for 6 hours. Two states of the alloy (coarse and fine grained) were used in present study. The coarse grained material had an initial size about 118 µm (state 1) and was produced by water quenching of the cast ingot from the standard homogenization temperature. The fine grained material had an initial grain size about 10 µm (state 2) and was produced by a
thermomechanical process. Samples were annealed at 500°C in a furnace for one hour and slow cooled after thermomechanical processing.
The microstructural evolution of the 2219 aluminum alloy during severe plastic deformation was evaluated in torsion using the Bridgeman anvil technique . Torsion samples, which were prepared from both states of the material, had a diameter of 8 mm and a thickness of 0.3 mm. These samples were deformed at ambient temperature and a pressure of 5 GPa was applied during torsional deformation. True strain ε was estimated by use of the expression
ε = ln(φd/2a) (1)
where φ is an angular displacement, d is the diameter of the tested sample and a is the thickness. The microhardness of the samples after various increments in torsional strain was evaluated using a PMT-3 device with a load of 20 g on Vickers diamond pyramid intentor. Samples were also examined using TEM. For these examinations, discs 3 mm in diameter were cut from the samples and then electropolished in a Tenupol-3 twin-jet polishing unit using a standard 30%CH3COOH+70%HNO3 solution at -30
0C. The thin foils were examined using a Jeol-2000EX TEM and a double-tilt stage with an accelerating potential of 200 kV. X-ray analysis was performed using a DRON-4 device. The coherent domain size and internal elastic strain were determined using the Williamson-Hall method.
The microhardness of the as-processed samples is shown in Fig. 1 as a function of strain. Up to ε = 0.5, the results show that, for both states of the material, plastic deformation does not produce significant increases in the hardness of the 2219 alloy. In the range ε = 0.5 - 2, the microhardness increases by approximately a factor of two. Above ε = 2, the microhardness increases gradually with the microhardness of state 2 increasing faster than the hardness of state 1. At ε ≤ 4, state 1 has a greater hardness than state 2; by ε = 7, the higher rate of increase in the hardness of state 2 causes the two states to have comparable microhardnesses.
0 1 2 3 4 5 6 7 8
State 2 State 1
Fig.1. Microhardness vs. strain for the two states of the 2219 aluminum alloy.
The results of the X-ray line broadening analysis are presented in Fig. 2 for strains greater than ε = 0.5. Both the coherent domain size and the internal elastic strain decrease with increasing strain. The largest decrease in both these quantities occurs in the strain range ε = 0.5 - 1. At a strain of ε = 1, the coherent domain size has decreased to 0.09 µm for the material in state 1 and 0.15 µm for the material in state 2. Relatively insignificant reductions in coherent domain size and internal elastic strain occur at strains larger than ε = 1.
0 1 2 3 4 5 6 7 8
State 1 State 2
0 1 2 3 4 5 6 7 8
State 2 State 1
Fig.2. Coherent domain size (a) and internal elastic strain (b) vs. strain for the two states of the 2219 aluminum alloy.
Examination of the deformed samples using TEM showed that after a strain of ε = 0.5 a cell structure had developed (Fig. 3a). This cell structure was observed for both states of the material and consisted of cells bounded by banded areas of uniform diffraction contrast containing a high density of lattice dislocations. These volume elements had an average size of about 1 µm and a boundary thickness of about 500 nm. Inside the cells, tangled dislocations were observed with a lower dislocation density than in the boundaries. Diffraction analysis revealed spots that were elongated in the azimuthal direction by 1-30. These elongated spots are indicative of continuous misorientations in the cell structure. Increasing plastic deformation produces a change in the cell structure. The conventional cell structure  transforms into a lamellar band (LB) structure . This lamellar structure consists of misoriented high density dislocation bands. This structure is similar to the cell block structure reported by Bay et al.  and Hughes and Hansen . In addition, there were highly misorientated areas within the LBs. Observation of Moire patterns inside of the LBs also indicated that progressive misorientation exists within the bands. It was evident from diffraction contrast that there was misorientation between a LB boundary and LB body. A reduction of the LB boundary thickness to about 300 nm (Fig. 3b) was observed at ε= 1 relative to cell boundary thickness at e=0.5. In addition the dislocation density within the cel